advertisement

COMPOSITES SCIENCE AND TECHNOLOGY Composites Science and Technology 67 (2007) 2941–2946 www.elsevier.com/locate/compscitech The eﬀect of van der Waals-based interface cohesive law on carbon nanotube-reinforced composite materials H. Tan a,* , L.Y. Jiang b, Y. Huang c, B. Liu d, K.C. Hwang d a School of Mechanical, Aerospace and Civil Engineering, University of Manchester, Manchester, M60 1QD, UK Department of Mechanical and Materials Engineering, University of Western Ontario, London, ON N6A 5B9, Canada Department of Mechanical Science and Engineering, University of Illinois at Urbana-Champaign, Urbana, IL 61801, United States d Department of Engineering Mechanics, Tsinghua University, Beijing 100084, China b c Available online 18 May 2007 Abstract The nonlinear cohesive law derived from the weak van der Waals force for carbon nanotube/polymer interfaces is incorporated in present study of CNT-reinforced composites. Carbon nanotubes can indeed improve the mechanical behavior of composite at the small strain, but such improvement disappears at relatively large strain because the completely debonded nanotubes behave like voids in the matrix and may even weaken the composite. The increase of interface adhesion between carbon nanotubes and polymer matrix may signiﬁcantly improve the composite behavior at the large strain. 2007 Elsevier Ltd. All rights reserved. Keywords: C. van der Waals force; B. Fibre/matrix bond; A. Carbon ﬁbres; B. Interface; A. Polymer-matrix composites (PMCs) 1. Introduction Carbon nanotubes (CNT) display superior mechanical properties, and are an excellent candidate of reinforcements for nanocomposites [1,2]. The CNT-reinforced composites, however, never reach their expected mechanical properties [3]. This has triggered signiﬁcant research eﬀorts to understand this shortfall and to improve the mechanical properties of CNT-reinforced nanocomposites [4–9]. Nanocomposites possess a large amount of interfaces due to the small (nanometer) size of reinforcements. The interface behavior can signiﬁcantly aﬀect the mechanical properties of nanocomposites. For example, carbon nanotubes in general do not bond well to polymers [10–12], and their interactions result mainly from the weak van der Waals forces [13–17]. Consequently CNTs may slide inside the matrix and may not provide much reinforcing eﬀect. It is, however, important to assess whether the poor interface behavior is * Corresponding author. Tel.: +1 217 244 4799; fax: +1 217 244 6534. E-mail address: [email protected] (H. Tan). 0266-3538/$ - see front matter 2007 Elsevier Ltd. All rights reserved. doi:10.1016/j.compscitech.2007.05.016 indeed responsible for the short fall of CNT-reinforced composites in order to reach their expected properties. It is diﬃcult to account for the van der Waals interactions in the continuum modeling of nanocomposites. Jiang et al. [2] established a nonlinear cohesive law for the CNT/ polymer interfaces directly from the Lennard–Jones (LJ) potential for the van der Waals interactions. The cohesive law gives analytically the normal cohesive stress at the CNT/polymer interface, rint, in terms of the interface opening displacement [u]. The normal cohesive stress rint displays nonlinear hardening, peak strength, and softening behavior as the opening displacement [u] increases. All cohesive law properties (e.g. cohesive strength, cohesive energy) are obtained analytically in terms of the parameters in the LJ potential. The objective of this paper is to incorporate Jiang et al.’s [2] nonlinear cohesive law for CNT/polymer interfaces in the study of the macroscopic behavior of CNT-reinforced composites. It provides a direct link between the macroscopic behavior of nanocomposites and the nanoscale behavior of interfaces, and therefore an assessment H. Tan et al. / Composites Science and Technology 67 (2007) 2941–2946 whether the interface behavior is indeed responsible for the macroscopic properties of nanocomposites. The paper is outlined in the following. The nonlinear cohesive law [2] for CNT/polymer interfaces is summarized in Section 2. A micromechanics model is provided in Section 3 to predict the nonlinear behavior of CNT-reinforced composite in terms of the properties of CNT/matrix interfaces, as well as those of CNTs and matrix. An example of a CNT-reinforced composite subjected to hydrostatic tension is used to illustrate the eﬀect of nonlinear cohesive law. The nonlinear stress–strain curve of the CNT-reinforced composite is given in Section 4. 2. A nonlinear cohesive law for carbon nanotube/polymer interfaces The energy between two atoms of distance r due to the van der Waals force can be represented by the LJ 6–12 potential, 12 r r6 V ðrÞ ¼ 4e 12 6 ; ð2:1Þ r r pﬃﬃﬃ where 6 2r is the equilibrium distance between atoms, and e is the bond energy at the equilibrium distance. For the van der Waals interaction between a carbon atom and a –CH2– unit of polyethylene, e = 0.004656 ev and r = 0.3825 nm [18]. Based on the LJ potential for the van der Waals interaction, Jiang et al. [2] established the following cohesive law for CNT/polymer interfaces, " 4 rmax int r ¼3:07rmax 1 þ 0:682 ½u Utotal 10 # rmax 1 þ 0:682 ½u ; ð2:2Þ Utotal int where r and [u] are the normal cohesive stress and opening displacement at the CNT/polymer interface, respectively, the cohesive strength rmax and total cohesive energy Utotal are related to the parameters r and e in LJ potential in Eq. (2.2) by rmax 6p q q er2 ¼ 5 p c and Utotal 4p ¼ 9 rﬃﬃﬃ 5 q q er3 : 2 p c ð2:3Þ ð2:4Þ Here qc is the CNT area density (number of carbon atoms per unit area of CNT) which equals 3.82 · 1019 m2 [19], qp is the polymer volume density (number of polymer molecules per unit volume). For the –CH2– unit in polyethylene, qp can be obtained from the ratio of polyethylene mass density 0.71 · 103 kg m3 [18] to the mass of –CH2– unit (2.3 · 1026 kg) as qp = 3.1 · 1028 m3. Eq. (2.3) then gives a rather high cohesive strength, rmax = 479 MPa, as compared to the Young’s modulus of polyethylene (0.9 GPa). 500 450 400 cohesive stress (MPa) 2942 350 300 cohesive energy=0.107J/m2 250 200 150 100 50 0 0 0.25 0.5 0.75 1 interface opening (nm) Fig. 1. The cohesive law for a carbon nanotube and polymer matrix established from the van der Waals interactions at the nanotube/matrix interface. The normal cohesive stress rint is shown versus the interface opening displacement [u] for a carbon nanotube and polyethylene matrix. However, Eq. (2.4) gives a very low cohesive energy Utotal = 0.107 Jm2, which is consistent with the poor bonding between CNTs and polymer. Fig. 1 shows the normal cohesive stress rint versus the interface opening displacement [u]. The cohesive stress increases rapidly at small opening displacement, reaches the cohesive strength at [u] = 0.0542 nm and then gradually decreases as [u] increases. The overall area underneath the curve is the total cohesive energy, 0.107 Jm2. 3. A micromechanics model for nanocomposites with nonlinear interface cohesive law We ﬁrst consider a composite material with long ﬁbers since CNTs have very large aspect ratio (e.g. 105). The ﬁber volume fraction is denoted by f. 3.1. Macroscopic strain of the nanocomposite and strain e of the nanocomThe macroscopic stress r posite represent the collective, homogenized behavior of ﬁbers and matrix. They are distinguished from the microscopic stress r and strain e in ﬁbers and matrix since the latter satisfy the constitutive laws in the corresponding constituents, and are nonuniform due to the material inhomogeneities. The macroscopic strain is given by [20,21] e ¼ M m : r þ f ðM f M m Þ : rf þ eint ; ð3:1Þ where the matrix and ﬁbers are linear elastic with the elastic compliance tensor Mm for the matrix and Mf for ﬁbers; hrfiis the average stress in ﬁbers; and heintirepresents the contribution from the ﬁber/matrix interface and is given by Z int 1 e ð½u n þ n ½uÞdA: ð3:2Þ ¼ 2Xf S int H. Tan et al. / Composites Science and Technology 67 (2007) 2941–2946 Here Xf is the total ﬁber volume, and Sint represents all ﬁber/matrix interfaces. For perfectly bonded interfaces, heinti = 0. For not-well-bonded interfaces as in CNT-reinforced composites, he inti and hrfi are to be determined from the interface cohesive law. We consider a simple case of an isotropic matrix containing randomly distributed, long and isotropic ﬁbers subI, where I is the second-order jected to hydrostatic tension r identity tensor. The macroscopic strain of the composite is eI and e is obtained from Eq. (3.1) as f int 1 f 1 1 e ¼ þ r rkk þ ekk ; ð3:3Þ 3 Km 3 3 Kf 3 Km where Km and Kp are the elastic bulk moduli of the matrix and ﬁbers, respectively, and eint kk is related to the displacement jump [u] in the normal direction across the ﬁber/matrix interface by Z int 1 ekk ¼ ½udA: ð3:4Þ Xf S int For the nonlinear cohesive law in Section 2, the displacement jump [u] is related to the normal cohesive stress rint via Eq. (2.2). A micromechanics model, such as the dilute f solution int in the next section, is needed to determine rkk (or eÞ. Eq. (3.3) then gives the nonand ekk in terms of r linear stress–strain relation. 3.2. Dilute solution Since, the CNT volume fraction is small, we may use the dilute solution which neglects the interactions among ﬁbers. Consider a long ﬁber of radius R in an inﬁnite matrix sub and e denote jected to remote hydrostatic tension. Let r the macroscopic stress and strain of the composite, and rint the normal cohesive stress at the ﬁber/matrix interface. The stresses in the ﬁber are uniform, rfrr ¼ rfhh ¼ rint ¼ constant, and rfzz ¼ constant, where (r,h,z) are the cylindrical coordif f nates. The strains in the f ﬁber are err ¼ ehh ¼ ½ð1 mf Þ int f f int r mf rzz =Ef and ezz ¼ rzz 2mf r =Ef , where Ef and mf are the Young’s modulus and Poisson’s ratio of the ﬁber. The radial displacement at the ﬁber boundary is R ð1 mf Þrint mf rfzz =Ef . The matrix stress in the ﬁber direction is the same as . The radial displacement in the matrix macroscopic stress r takes the form ur = Ar+B/r [22], where the coeﬃcients A and B are to be determined by the remote boundary condim int tion rm ¼ r and the interface condition r rr r!1 rr r¼R ¼ r . The displacement at the ﬁber/matrix interface r = R is then given by R½ð2 mm Þ r ð1 þ mm Þrint =Em , where Em and mm are the Young’s modulus and Poisson’s ratio of the matrix, respectively. The opening displacement is the displacement jump across the ﬁber/matrix interface, i.e. R R ½u ¼ ð2 mm Þ r ð1 þ mm Þrint ð1 mf Þrint mf rfzz Em Ef ð3:5Þ 2943 It is recalled that the normal cohesive stress rint = r int([u]) is related to the opening displacement [u] via the nonlinear cohesive law (2.2). Eq. (3.5) then gives the macroscopic in terms of [u] and rfzz , and rfzz is to be determined stress r by the Reuss approximation in the following. The macroscopic strain e can be obtained from Eq. (3.3). For very long ﬁbers, Reuss approximation [23] gives the ﬁber stress rfzz in the ﬁber direction to be the same as the macroscopic stress : rfzz ¼ r ð3:6Þ The Reuss approximation, however, gives a lower bound solution and underestimates the reinforcing eﬀect of ﬁbers. f int . The addi¼ 2r þr The average stress in ﬁber is r kk due to interface opening is 2[u]/R. Eq. tional strain eint kk (3.5) gives the macroscopic stress in terms of the interface opening displacement [u] as ½u m f þ 1þm þ 1m rint ð½uÞ Em Ef R ¼ r ; ð3:7Þ 2mm þ Emff Em where rint([u]) is obtained from Eq. (2.2). The macroscopic strain is obtained in terms of [u] from Eq. (3.3) as int 1 f 1 1 ½u e ¼ þ2 þ r : 2r ð½uÞ þ r 3 Km 3 3 Kf 3 Km R ð3:8Þ and strain Eqs. (3.7) and (3.8) give the macroscopic stress r e in terms of [u] based on the Reuss approximation, and therefore provide the nonlinear stress–strain relation of the CNT-reinforced composite. 4. Stress–strain curve of CNT-reinforced composite The CNT Young’s modulus Ef is on the order of 1 TPa [24], which is several orders of magnitude higher than the modulus Em of polymer matrix (e.g. 0.9 GPa for polyethylene). (The CNT elastic modulus in the CNT radial direction may be smaller than that in the axial direction, but is still much larger than the polymer modulus.) For Ef Em, the stress–strain relation (3.7) and (3.8) is simpliﬁed to " 4 Em ½u 1 þ mm rmax ¼ þ 3:07 r rmax 1 þ 0:682 ½u 2 mm R 2 mm Utotal 10 # rmax 1 þ 0:682 ½u ; ð4:1Þ Utotal 1 2mm þ f ½u f 1 2mm rmax e ¼ þ 3:07 1 þ mm ð5 mm Þ 2 mm R 3 2 mm E m " 4 10 # rmax rmax 1 þ 0:682 ½u 1 þ 0:682 ½u ; Utotal Utotal ð4:2Þ where Eq. (2.2) has been used. Fig. 2 shows the stress–strain curve for a CNT-reinforced polyethylene composite subjected to hydrostatic ten- 2944 H. Tan et al. / Composites Science and Technology 67 (2007) 2941–2946 0.6 1% 0.6 5% matrix 0.5 0.5 armchair (18, 18) carbon nanotube f=10% 0.4 stress (GPa) stress (GPa) 0.4 armchair (18, 18) carbon nanotube f= 10% 0.3 0.2 0.1 0 0.3 0.2 0.1 0 0.05 0.1 0.15 0.2 0 0.25 strain sion. For comparison the straight line for the linear elastic polyethylene matrix is also shown. The polyethylene Young’s modulus and Poisson’s ratio are Em = 0.9 GPa and mm = 0.33, respectively. The nanotube radius is R = 1.25 nm for the armchair (18,18) CNTs. The CNT volume fraction is f = 10%. (It is well known that the dilute solution holds only for the small reinforcement volume fraction since it neglects the reinforcement interactions. Tan et al. [21] has shown that the dilute solution is diﬀerent from the Mori–Tanaka method, which accurately accounts for the reinforcement interactions, by a factor of 1 f. For CNT volume fraction f = 10%, this factor is 90%.) For strain less than 13.9%, the stress–strain curve is almost (but not exactly) a straight line that is above the straight line for the matrix and reﬂects the CNT reinforcing eﬀect. (The curve for the composite is not signiﬁcantly higher than the straight line for the polyethylene matrix because the Reuss approximation gives a lower bound solution and therefore underestimates the CNT reinforcing eﬀect.) Once the strain reaches 13.9% (and the stress reaches the peak strength 406 MPa), both stress and strain decrease due to the interface softening behavior displayed in the cohesive law (Fig. 1). The stress and strain start to increase again as the strain drops to 9.1%, but the curve becomes lower than the straight line for the matrix because the completely debonded CNTs are equivalent to voids and therefore weaken the matrix. For the displacement-controlled experiment, the stress–strain curve would drop vertically from 406 MPa to 289 MPa at the 13.9% strain, as illustrated by the arrow in Fig. 2, and then gradually increase. Fig. 3 shows the stress–strain curves for the polyethylene matrix with armchair (18,18) CNTs at three volume fractions, f = 1%, 5% and 10%. The peak strengths for diﬀerent 0.05 0.1 0.15 0.2 0.25 strain Fig. 3. The macroscopic stress–strain relation of a carbon nanotubereinforced polyethylene matrix composite. The volume fraction of armchair (18,18) carbon nanotubes is 10%, 5% and 1%. f are exactly the same, 406 MPa, such that the CNT volume fraction has no eﬀect on the composite strength. The critical strain at the peak strength changes slightly, 13.9% for f = 10%, 14.6% for f = 5% and 15.2% for f = 1%. The CNT volume fraction f = 10% gives a higher initial modulus than f = 5% (or 1%), but it also gives a lower incremental modulus at large strain (after CNTs are completely debonded). For the displacement-controlled experiment, the vertical stress drop is 117 MPa for f = 10%, and 68 MPa and 16 MPa for f = 5% and 1%, respectively. Therefore, CNTs may reinforce the composite at the small strain but weaken it at the large strain. 0.6 armchair carbon nanotube f= 10 % 0.5 (6 , 6) 0.4 stress (GPa) Fig. 2. The macroscopic stress–strain relation of a carbon nanotubereinforced polyethylene matrix composite subjected to hydrostatic tension. The volume fraction of armchair (18,18) carbon nanotubes is 10%. The linear elastic stress–strain relation of the polyethylene matrix is also shown. 0 ,12 (1 2 0.3 ( 18 0.2 , 18 ) ) 0.1 0 0 0.05 0.1 0.15 0.2 0.25 strain Fig. 4. The macroscopic stress–strain relation of a carbon nanotubereinforced polyethylene matrix composite. The volume fraction is 10% for three diﬀerent armchair carbon nanotubes (18,18), (12,12) and (6,6). H. Tan et al. / Composites Science and Technology 67 (2007) 2941–2946 Fig. 4 shows the eﬀect of CNT size on the stress–strain curve. The CNT volume fraction is ﬁxed at f = 10%. Three diﬀerent armchair CNTs, (18,18), (12,12) and (6,6), are examined, and the corresponding radii are R = 1.25, 0.83 and 0.42 nm, respectively. The peak strength increases from 406 MPa to 419 and 462 MPa as the CNT radius decreases, from (18,18) to (12,12) and (6,6). The critical strain for the peak strength also increases, from 13.9% to 14.6% and 16.8%. Small CNTs clearly give stronger reinforcing eﬀect than large CNTs because, at a ﬁxed CNT volume fraction, there are more small CNTs than large ones, and therefore more interfaces. This observation of strong reinforcing eﬀect for small CNTs also holds after CNTs are debonded from the matrix. The stress drop is 117 MPa, 106 MPa and 41 MPa for the (18,18), (12,12), and (6,6) CNTs. Therefore, small CNTs are more eﬀective than large CNTs. In order to investigate whether the interface bonding has a strong inﬂuence on the macroscopic behavior of CNTreinforced composites, we double and quadruple the total cohesive energy to Utotal = 0.214 Jm2 and 0.429 Jm2 while maintaining the same cohesive strength rmax = 479 MPa. Fig. 5 shows the stress–strain curve of the composite with f = 10% volume fraction of armchair (18,18) CNTs. The peak strength increases from 406 MPa to 432 and 496 MPa when the total cohesive energy changes from 0.107 Jm2 to 0.214 and 0.429 Jm2, respectively. The corresponding strain for the peak strength also increases from 13.9% to 15.3% and 18.9%. The overall stress–strain curve for large Utotal (0.429 Jm2) becomes much higher than that for low Utotal (0.107 Jm2). Therefore, strong adhesion between CNTs and polymer matrix may signiﬁcantly 0.6 2 armchair (18, 18) carbon nanotube f= 10 % 2 0.4 0.5 9J/ m 2 stre ss (GPa) 0.4 0 5 .21 J /m 0.3 Φ total = 0. 107J/ m 2 0.2 0.1 0 0 0.05 0.1 0.15 0.2 0.25 strain Fig. 5. The macroscopic stress–strain relation of a carbon nanotubereinforced polyethylene matrix composite. The volume fraction is 10% for armchair (18,18) carbon nanotubes. Three values of the total cohesive energy are taken, Utotal = 0.107, 0.214 and 0.429 Jm2. The cohesive strength is ﬁxed at 479 MPa. 2945 improve the mechanical behavior of CNT-reinforced composites. 5. Concluding remarks For carbon nanotubes not well bonded to polymers, Jiang et al. [2] established a cohesive law for carbon nanotube/ polymer interfaces. The cohesive law and its properties (e.g. cohesive strength, cohesive energy) are obtained directly from the Lennard–Jones potential from the van der Waals interactions. Such a cohesive law is incorporated in the micromechanics model to study the mechanical behavior of carbon nanotube-reinforced composite materials. Carbon nanotubes indeed improve the mechanical behavior of composite at the small strain. However, such improvement disappears at relatively large strain because the completely debonded nanotubes behave like voids in the matrix and may even weaken the composite. The increase of interface adhesion between carbon nanotubes and polymer matrix may signiﬁcantly improve the composite behavior at the large strain. Acknowledgement This research was supported by the ONR Composites for Marine Structures Program (Grants N00014-01-10205, Program Manager Dr. Y.D.S. Rajapakse). References [1] Thostenson ET, Chou TW. Aligned multi-walled carbon nanotubereinforced composites: processing and mechanical characterization. J Phys D: Appl Phys 2002;35:L77–80. [2] Jiang LY, Huang Y, Jiang H, Ravichandran G, Gao H, Hwang KC, et al. A cohesive law for carbon nanotube/polymer interfaces based on the van der Waals force. J Mech Phys Solids 2006;54:2436–52. [3] Baughman RH, Zakhidov AA, de Heerm WA. Carbon nanotubes– the route toward applications. Science 2002;297:787–92. [4] Thostenson ET, Ren ZF, Chou TW. Advances in the science and technology of carbon nanotubes and their composites: a review. Compos Sci Technol 2001;61:1899–912. [5] Thostenson ET, Li CY, Chou TW. Nanocomposites in context. Compos Sci Technol 2005;65:491–516. [6] Maruyama B, Alam H. Carbon nanotubes and nanoﬁbers in composite materials. SAMPE J 2002;38:59–70. [7] Deepak S, Wei C, Cho K. Nanomechanics of carbon nanotubes and composites. Appl Mech Rev 2003;56:215–30. [8] Breuer O, Sundararaj U. Big returns from small ﬁbers: a review of polymer/carbon nanotube composites. Polym Compos 2004;25: 630–45. [9] Harris PJF. Carbon nanotube composites. Int Mater Rev 2004;49:31–43. [10] Schadler LS, Giannaris SC, Ajayan PM. Load transfer in carbon nanotube epoxy composites. Appl Phys Lett 1998;73:3842–4. [11] Ajayan PM, Schadler LS, Giannaris C, Rubio A. Single-walled carbon nanotube-polymer composites: strength and weakness. Adv Mater 2000;12:750–3. [12] Lau KT, Shi SQ. Failure mechanisms of carbon nanotube/epoxy composites pre-treated in diﬀerent temperature environments. Carbon 2002;40:2965–8. 2946 H. Tan et al. / Composites Science and Technology 67 (2007) 2941–2946 [13] Liao K, Li S. Interfacial characteristics of a carbon nanotubepolystyrene composite system. Appl Phys Lett 2001;79: 4225–7. [14] Frankland SJV, Caglar A, Brenner DW, Griebel M. Molecular simulation of the inﬂuence of chemical cross-links on the shear strength of carbon nanotube-polymer interfaces. J Phys Chem B 2002;106:3046–8. [15] Li CY, Chou TW. Multiscale modeling of carbon nanotube reinforced polymer composites. J Nanosci Nanotechno 2003;3:423–30. [16] Wong M, Paramsothy M, Xu XJ, Ren Y, Li S, Liao K. Physical interactions at carbon nanotube-polymer interface. Polymer 2003;44:7757–64. [17] Gou J, Minaie B, Wang B, Liang Z, Zhang C. Computational and experimental study of interfacial bonding of single-walled nanotube reinforced composites. Comp Mater Sci 2004;31:225–36. [18] Frankland SJV, Harik VM, Odegard GM, Brenner DW, Gates TS. The stress–strain behavior of polymer-nanotube composites from [19] [20] [21] [22] [23] [24] molecular dynamics simulation. Compos Sci Technol 2003;63: 1655–61. Jiang H, Zhang P, Liu B, Huang Y, Geubelle PH, Gao H, et al. The eﬀect of nanotube radius on the constitutive model for carbon nanotubes. Comput Mater Sci 2003;28:429–42. Benveniste Y, Aboudi J. A continuum model for ﬁber reinforced materials with debonding. Int J Solids Struct 1984;20:935–51. Tan H, Huang Y, Liu C, Geubelle PH. The Mori–Tanaka method for composite materials with nonlinear interface debonding. Int J Plasticity 2005;21:1890–918. Timoshenko S, Goodier JN. Theory of Elasticity. Third ed. McGrawHill; 1970. Reuss A. Berechung der Fliessgrenze von Mischkristallenx auf Grund der Plastizitätsbedingung für Einkristalle. Z Angew Math Mech 1929;9:49–58. Huang Y, Wu J, Hwang KC. Thickness of graphene and single-wall carbon nanotubes. Phys Rev B 2006;74:245413.